# Evidence of the contribution of molecular fluorophores to the luminescence of carbon entities formed by solvothermal treatment of trinitropyrene

Rayan Roch, Xavier Deschanels, Chandra Mohan Singaravelu, Noé André, Cyrielle Rey, Jérémy Causse

<figure><img src="image_1.png" /></figure>

## To cite this version:

Rayan Roch, Xavier Deschanels, Chandra Mohan Singaravelu, Noé André, Cyrielle Rey, et al. Evidence of the contribution of molecular fluorophores to the luminescence of carbon entities formed by solvothermal treatment of trinitropyrene. RSC Advances, 2024, 14 (54), pp.39858-39866. 10.1039/d4ra07553f. hal-04848736

HAL Id: hal-04848736

https://hal.science/hal-04848736v1

Submitted on 16 May 2025

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_2.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
<figure><img src="image_3.png" /></figure>

Check for updates

Cite this: RSC Adv., 2024, 14, 39858

# Evidence of the contribution of molecular fluorophores to the luminescence of carbon entities formed by solvothermal treatment of trinitropyrene†

Rayan Roch, ID* Xavier Deschanels, ID* Chandra Mohan Singaravelu, Noé André, Cyrielle Rey ID and Jérémy Causse ID*

Carbon dots are a subset of carbon nanomaterials with fluorescent properties that render them attractive for various potential applications such as bioimaging and sensing. The past years saw significant progress being made in the understanding of the formation and the underlying fluorescent property. Nevertheless, efforts are still necessary to unravel the formation of carbon dots and the origin of their luminescence, especially for new types of precursor material such as polycyclic aromatic compounds. Trinitropyrene, a nitroaromatic derivative of pyrene, is increasingly being used as an organic precursor for carbon dot synthesis by bottom-up method. This work aims to study the luminescent products obtained by microwave-assisted solvothermal treatment of trinitropyrene in a common organic solvent for nanoparticle synthesis, dimethylformamide. By employing flash chromatography, we isolated different fractions from which mainly stems the fluorescence observed from the crude sample obtained post solvothermal treatment. By performing structural and spectroscopic characterization techniques, we observed that they possess quiet similar chemical composition and luminescent properties but significant differences from a structural point of view. From these observations, we suggest that the fractions mainly consist of molecular derivatives of the precursor material. This study calls attention to the need of separation and purification techniques in order to better assess the properties of carbon dots.

Received 22nd October 2024
Accepted 11th December 2024

DOI: 10.1039/d4ra07553f

rsc.li/rsc-advances

## Introduction

Carbon dots (CDs) are a subset of fluorescent carbon nanomaterials serendipitously discovered in 2004 during the purification of single-walled carbon nanotubes.¹ They display remarkable physicochemical properties such as photoluminescence, solubility in aqueous and/or organic media,²⁻⁴ and photostability as well as potential fields of application like bioimaging,⁵,⁶ sensing⁷⁻⁹ and optoelectronics.¹⁰⁻¹² There is a growing interest in these nanoparticles due to the simplicity of their synthesis protocol and the accessibility of precursors, leading to the publication of many articles in recent years. Carbon dots are defined by a characteristic size of less than 10 nm and a quasi-spherical shape. These nanoparticles consist of a predominantly carbon core with amorphous and crystalline areas along with chemical groups on the surface. Carbon dot synthesis approaches can be separated in two categories: bottom-up and top-down synthesis. In the top-down approach,

other carbon allotropes are fragmented to attain the desired nanoparticles through laser ablation, arc discharge, electrochemical,¹³⁻¹⁵ and acidic treatment. In the bottom-up approach, the nanoparticles are built from small organic molecules that undergo treatments such pyrolysis, microwave, and solvothermal treatments. Bottom-up synthesis of carbon dots has seen great progress in particular. Most of the attention is directed on citric acid systems and a few aromatic compounds such as phenylene diamine and phenolic derivatives.¹⁶ However, recent works highlighted the formation of fluorophores of citrazinic acid derivatives in citric acid systems. Moreover, methods of purification and separation are often insufficient or inadequate, if any at all. Formation of molecular fluorophores and inadequate purification methods leads to properties misattributed to carbon dots and is detrimental for the better understanding of these nanoparticles. Polycyclic aromatic compounds are increasingly used as precursors for bottom-up synthesis. They possess large conjugation domains, an attractive feature for some optical properties such as NIR fluorescence.¹⁷ Trinitropyrene (TNP) is a reactive pyrene derivative that is being growingly reported in recent years as a precursor for CDs synthesis.¹⁸⁻²⁹ Wang *et al.* reported the first synthesis of carbon dots involving trinitropyrene as the

<footnote>ICSM, University Montpellier, CEA, CNRS, ENSCM, 30207 Marcoule, France. E-mail: rayan.roch@gmail.com; xavier.deschanels@cea.fr; jeremy.causse@cea.fr
† Electronic supplementary information (ESI) available. See DOI: https://doi.org/10.1039/d4ra07553f</footnote>
precursor.¹⁸ Graphene quantum dots (GQDs) with remarkable crystallinity and optical properties were described in the literature, as a type of CDs composed of one or a few nanosized graphene layers stacked that display well-ordered morphology. Wang and his coworkers presented a room temperature synthesis of GQDs *via* electron-beam radiation and a demonstration of its application as a fluorescent probe for cell imaging. Wu *et al*. reported organic soluble carbon dots with high mass yield.²⁰ They display long wavelength emissions and high solubility in a wide range of polar and non-polar solvents. Trinitropyrene was also employed jointly with various co-precursors such as boric acid,²⁴,²⁵,²⁷,²⁹ polyethylene-imine,²³ 2,4-diaminobenzenesulfonic acid,²⁸ diethylenetriamine²⁶ and in different solvents.²¹ However, despite of the increasing numbers of articles employing trinitropyrene as a precursor, studies on the structural and emissive properties of TNP-derived C-Dots were only recently addressed. Batra *et al*. investigated three fluorescent components in CDs from TNP.³⁰ Using a series of separation techniques, they showed that the sample was constituted with components with different weight percentages in the synthesis mixture and different quantum yield (QY). The isolated components presented distinct chemical and optical properties. They suggested that the fraction with the highest QY and mainly responsible for the observed emission corresponds to molecular fluorophore in the form of pyrene derivatives. They also came to the conclusion that the fraction with the second highest QY displays a quasi-CNDs like structure and the fraction with the lowest QY is the one the exhibiting coherent structural properties with what is expected from CDs. CNDs are defined as a type of CDs with a varying proportion of amorphous and ordered carbon in a sphere-like shape. Kothalawala *et al*. studied the nature and properties emissive components produced through hydrothermal treatment of TNP.³¹ They isolated small molecular fluorophores with clearly different chemical structure and optical properties significantly brighter emission than the CDs obtained in the same synthesis. Batra and Kothalawala both showed that the constituents of the mixture obtained after hydrothermal treatment were of different nature and showed distinct optical properties compared to the CDs produced simultaneously/alongside. Most of them displayed significantly brighter emission than CDs. Nonetheless, they both worked in specific hydrothermal conditions. Even if numerous reports of synthesis based on trinitropyrene in organic solvents have been made, the synthesis was never investigated in organic medium to such an extent to our knowledge. Hence, this study is focused on the solvothermal treatment of TNP in dimethylformamide (DMF), a commonly used organic solvent used in solvothermal synthesis, in order to investigate the nature and properties of the fluorescent constituent obtained in these conditions.

## Experimental

### Materials and methods

All chemicals and solvents used were purchased from commercial suppliers and used without further purification as follows. Nitric acid (ACS reagent, 69%), sulfuric acid (RPE,

96%), N,N'-dimethylformamide (ACS reagent, ≥99.8%), ethanol (RE grade), cyclohexane (RPE grade), dichloromethane (RE grade), methanol (RE grade), NaOH were purchased from Carlo Erba. Pyrene was purchased. Milli-Q water was used during the experiment. Flash chromatography was performed on a Rev eleris X2 flash chromatography system from BUCHI using 25 g Flashpure Ecoflex column containing 50 µm irregular silica. Dialysis membranes (regenerated cellulose, 1 kDa MWCO) were purchased from Spectra/Por.

### Synthetic procedures

Solvothermal treatment of TNP. The procedure to obtain trinitropyrene was based on a method proposed in the litter- ature²⁰ In a 500 ml-round bottom flask, 60 ml of HNO₃ and 20 ml of H₂SO₄ were mixed. 1 g of pyrene was added and the mixture was heated at 80 °C under stirring (750 rpm) for 48 hours. The flask was opened twice a day in order to eliminate the reddish fumes generated during the synthesis. After cooling to room temperature, 300 ml of water was slowly added. The mixture in flask was collected in centrifugation tubes. Following the centrifugation of the tubes, the supernatant was discarded, fresh water was added and the precipitate was redispersed. This operation was repeated until the pH of the supernatant after centrifugation was neutral. The resultant powder (1.44 g) was dried in an oven at 60 °C overnight and assumed to be TNP.

In a 35 ml vial containing 100 mg of TNP, 10 ml of DMF was added. The mixture was heated in a CEM Discover SP microwave system at 300 W and 200 °C under high stirring during deter- mined duration (20 min, 40 min, 60 min). After cooling to room temperature, a solvent exchange was performed during 6 hours using a semi-permeable membrane (regenerated cellulose, 1 kDa) to replace DMF with EtOH. The dialysate was replaced every two hours. The solution containing the sample in the dialysis tube was retrieved for further purification. Centrifugation ultrafiltra- tion was performed on the sample with a centrifugal filter (Vivaspin 15R, 2 kDa) at 4000 rpm at 35 °C during 1 h. The filtrate was discarded, ethanol was added to the filter device. The oper- ation was repeated until the filtrate was almost clear. The sample was retrieved and dry-loaded on silica gel for further purification. Flash chromatography was performed through a Puriflash system with a binary solvent mixtures cyclohexane/dichloromethane, respectively solvent A and B. A linear gradient elution method was executed as follows: a volume ratio of 50% of B, hold it for 3 column volumes (CV); 50% to 100% of B over 10 CV; 100% of B, hold it for 3 CV. In an attempt to collect a part of the sample that was barely eluting, another step with 90:10 ratio of dichloro- methane : methanol was added afterward, for 5 column volumes. Silica gel columns of 24 g were used as the stationary phase and equilibrated with 6 column volumes of 50% of each solvent. After collecting the tubes, the corresponding fractions were reas- sembled each in a round-bottom flask. The eluting mixture was removed using a rotary evaporator. Because the sample was spread in the flask, a small volume of acetone was added, the flask was rotated by hand in a sonicating in order to collect all the sample spread on the wall of the flask. The sample was then dried in an oven at 40 °C overnight.
## Characterization

Chemical structures and optical properties were obtained by X-ray diffraction analysis (XRD), Raman spectroscopy, Fourier transform infra-red spectroscopy (FTIR), UV-visible spectroscopy (UV-vis), High Resolution Mass Spectrometry (HRMS), Fluorescence spectroscopy, Scanning Electron Microscopy (SEM). UV-vis absorbance measurements of the fractions obtained by column chromatography in toluene were carried out using a Shimadzu UV-3600 spectrophotometer. The spectra were collected using a quartz cuvette with a 10 mm path length and a 3 ml volume. The samples were scanned in the wavelength range of 300–800 nm with a bandwidth of 3 nm and 1 s integration time. Emission spectra of the samples were recorded using a Horiba Scientific FluoroMax-4. The measurements were performed at a series of excitation wavelengths using a 2 nm entrance and 1 nm exit slits with an integration time of 0.1 s. 3D fluorescence mapping spectra were recorded in the excitation wavelength range of 250–600 nm and emission wavelength range of 550–700 nm. The value of the entrance and exit slit widths used were 1 nm for the column fractions and 2 nm for the TNP. Fourier transform Infrared (FTIR) spectra were recorded using a PerkinElmer IR-FT100 spectrometer equipped with an attenuated total reflection (ATR) module. The scans were recorded with a resolution 4 cm⁻¹ of and 10 repeated scans. The samples were placed in powder form on the ATR plate. Raman spectra were measured using a confocal microscope Raman LabRAM Aramis spectrometer equipped with a 532 nm excitation. The samples were placed in powder form on a glass plate. Diffraction patterns were recorded on a Bruker D8 Advance diffractometer using a Cu Kα radiation source, from 5° to 70°. SEM images were taken with a FEI QUANTA 200 ESEM

FEG microscope. HRMS was conducted using a Orbitrap ID-X (Waters) device and dichloromethane was used as the solvent. Samples were ionized following Electrospray Ionization technique (ESI).

The quantum yield values were measured with respect to the standard Fluorescein reference in 0.1 M NaOH using the slope method. The QY value of each sample was subsequently obtained using the following equation:

$$ \phi_X = \phi_S \left( \frac{\text{Grad}_X}{\text{Grad}_S} \right) \left( \frac{\eta_X^2}{\eta_S^2} \right) $$

where the subscripts S and X denote standard and sample respectively, Φ is the fluorescence quantum yield, Grad is the gradient from the plot of integrated fluorescence intensity vs. absorbance, and η is the refractive index of the solvent.

## Results and discussion

### Solvothermal treatment of TNP

The solvothermal treatment of nitrated pyrene-derived CDs was done using a microwave synthesizer (Fig. 1(a)). TNP was heated with DMF as the solvent under pressure as described in the experimental procedure section. After solvothermal treatment, the mixture is black opaque with dark reddish highlights. A solvent exchange step was performed in order to replace DMF, a high boiling point solvent with ethanol. This method allows the removal of DMF without heating the mixture. Indeed, further reactions could occur because of additional heating. The low CDs solubility in ethanol and results in an only small quantity of the sample thrown away with the DMF-containing ethanol eliminated. CDs obtained from trinitropyrene have

<figure><img src="image_4.png" /><figcaption>Fig. 1 (a) Schematic of the microwave-assisted solvothermal treatment of trinitropyrene in dimethylformamide. (b) Chromatogram of a sample (c) relative quantum yield for a given fraction depending on the synthesis duration (d) product yield for a given fraction depending on the synthesis duration.</figcaption></figure>

<figure><img src="image_5.png" /></figure>
been reported to display good solubility in low polarity
solvents.²¹ Ultrafiltration was performed in order to separate the
products from smaller molecular weight impurities. The
powder obtained was black and corresponded to a 90% mass
yield for the synthesis. It displayed a low solubility in ethanol
with a faint emission and good solubility in low polarity
solvents such as toluene with an orange-red emission. In order
to gain information on the sample obtained, silica column
chromatography was executed (Fig. 1(b) and S.I.A†). Several
fractions were obtained after this step labelled as F₁, F₂, F₃, F₄
and F₅ according to their eluting order. The duration of reten-
tion increases from F₁ to F₄ and F₅ eluting afterward in different
elution conditions due to the fact that this fraction was kept in
the stationary phase after the initial step of elution. Their
different retention times are due to their interactions with the
stationary phase, the silica. This stationary phase is a normal
phase of general purpose which tends to bind highly polar
compounds. The increasing retention times is attributed to an
increasing polarizability of the fractions.

The solvothermal treatment was performed at three different
durations (20 min, 40 min and 60 min) in order to investigate
a possible kinetic effect on the products. The quantum yield
values of all fractions are displayed in the Fig. 1(c). Overall, the
fractions exhibit QY values around 20% taking into account the
uncertainty of the relative quantum yield method. There is no
specific trend in the evolution of the quantum yield depending
on the duration of the synthesis. Depending on the eluting
order, the first and second fraction seems to exhibit a slightly
higher quantum yield compared to the other fraction. However,
compared to what Batra *et al.* and Kothalawala *et al.* reported,
the variation is hardly significant. We note first that we don't
obtain the same number of fractions. Indeed, whereas they both
obtained three main fractions, we obtained five fractions. Batra
*et al.* and Kothalawala *et al.* obtained respectively QY values of
12% and 31% for their first eluting fraction, 8% and 23% for
their second eluting fraction and 0.8% and 1% for their last
eluting fraction. The product yield values of the fractions are
also displayed in the Fig. 1(d). The product yield of the fractions
is in general around each 10%. A significant part of the other
half barely migrates during the column chromatography step
and stays stuck to the silica stationary phase. Since no signifi-
cant variations were observed regarding the quantum and mass
yields, we will focus on the synthesis carried out at a duration of
60 min from hereon.

Raman, FTIR, HRMS

To obtain more insight on the weight of the different fractions,
high resolution mass spectrometry was performed (see S.I.B/†).
Electrospray ionization-mass spectrometry was executed in both
positive and negative mode. Overall, in positive mode, the
spectra of the different fractions present a pseudo molecular
ion with a similar *m/z* mass around 415-420. Several peaks are
in common between the different fractions in addition to the
molecular pseudo-ions. Some peaks correspond to mono-
charged adducts with different ions (Na⁺, NH₄⁺, K⁺) commonly
observed in positive mode ESI-MS spectra (see Table S.I.B/1 and

Fig. S.I.B/2 from ESI†). Less intense peaks of lower or higher *m/z*
values are attributed to multimers and multicharged adducts.
The peaks at *m/z* 336 correspond to traces of TNP given that
M(TNP) = 337 g mol⁻¹. When the pseudo molecular ion [M + H]⁺
has the value *m/z* = 415, the peaks at 432 and 437 are
attributed to the monocharged adducts [M + NH₄]⁺ and [M + Na]⁺
respectively. The peaks at *m/z* = 846 are assigned [2M + NH₄].
When the pseudo molecular ion [M + H]⁺ has the value *m*
/*z* = 420, the peaks at 437 and 442 are attributed to the mono-
charged adducts [M + NH₄]⁺ and [M + Na]⁺ respectively. The
peaks at *m/z* = 856 are attributed to the multimer [2M + NH₄].
The results obtained in negative mode are slightly different. The
*m/z* values of the different fractions do not vary a lot between
themselves with values around 352 to 382. Other notable
intense peaks can be observed for *m/z* values of 309, 380 and
even 410. We observed the fact that the values in positive mode
are on average higher than in negative mode. We made the
hypothesis that an adduct might form between derivatives of
the precursor material and another compound such as
dichloromethane or dimethylformamide and that it might be
more easily detected in positive mode. It has to be noted that, in
positive mode, if we subtract 84 (ca. the value of the molar mass
of dichloromethane, the solvent used during the mass spec-
trometry analysis from the *m/z* values of the peaks considered to
be originating from the pseudo molecular ion (ca. 415 or 420),
we obtain values around 331 and 336. Moreover, in negative
mode, subtracting 73 (ca. the value of the molar mass of
dimethylformamide), from peaks with *m/z* values around 410,
426 or 442 yields values around 337, 353 and 369 which are close
to more intense peaks detected. Peaks at around *m/z* = 337 were
detected again. Overall, most of the *m/z* values detected vary
between 279 and 420. This suggests that these fractions are
mainly be composed of various nitropyrene derivatives.

FTIR spectroscopy was performed in an attempt to better
assess the chemical compositions of the samples (Fig. 2(a) and
S.I.C/†). Overall, the spectra of different fractions display
intense peaks in the 750–1600 cm⁻¹ region and smaller peaks
between 2800 and 3200 cm⁻¹. The fractions have several over-
lapping peaks in common with the spectrum of TNP, which
indicates similarities from a structural point of view. The
intensities of the peaks are not significantly different for the
main ones. The intense peaks around 1516 and 1346 are
attributed to the asymmetric and symmetric stretching of the
NO₂ bond respectively. These intense peaks present in every
FTIR spectra including the TNP, which suggest that the sample
still contains significant nitro group. Additionally, the fractions
show peaks corresponding to aromatic sp³ C–H stretching
(3100), C–H stretching (2920 cm⁻¹), C=C stretching (1590
cm⁻¹) and NO₂ shearing (860 cm⁻¹). We notice the absence of
broad intense hydroxyl peaks (around 3400 cm⁻¹). In order to
probe the chemical structure of the samples, the samples and
precursor were analysed by Raman spectroscopy (Fig. 2(b) and
S.I.D†). The acquisition of Raman spectra was negatively
impacted by the intense fluorescence in the background. The
Raman excitation laser causes damage to the sample because of
the localized heat. Laser attenuators were used in order to
diminis this effect. Raman spectra of carbon dots are expected

<figure><img src="image_6.png" /></figure>
<figure><img src="image_7.png" /></figure>

<figure><img src="image_8.png" /><figcaption>Fig. 2 (a) FTIR spectra of the fractions and the trinitropyrene (b) Raman spectra of the fractions and trinitropyrene.</figcaption></figure>

to display two bands in particular: the D band (1360 cm⁻¹) and the G band (1590 cm⁻¹). They correspond respectively to the amorphous sp³ hybridized carbon and the ordered sp² hybridized carbon in the material. Overall, the Raman spectra of the different fractions present intense large bands in common. Most of the intense ones are in common with TNP. The bands at 1590 cm⁻¹ and 1279 cm⁻¹ can be attributed to NO₂ asymmetric stretching and symmetric stretching. The bands in the range 1000–1300 cm⁻¹ are associated to CH in-plane bending vibrations. Overall, the FTIR results are consistent with the Raman results, a further indication that the fractions are close to TNP in terms of chemical groups.

Structural analysis (XRD, SEM)

Before purification, the diffractogram of the raw samples exhibits a pattern similar to what is expected from carbon dots (Fig. 3(a)). A large peak around 25° is observed with no particular sharp peaks that could be attributed to a quantity of fluorophores or other by-products. However, the fractions obtained after purification display different diffraction pattern from the raw sample (Fig. 3(b)). The Fig. S.I.E.† contains the diffraction patterns of the fractions with and without the background. The fractions are also compared between themselves for a given duration or for a given fraction Fₙ (see ESI†). For a synthesis of 60 minutes, F₁, F₂ and F₄ show sharp peaks between 5° and 40° and no large peak around 25° whereas F₃ has a small sharp peak

at 2θ < 10° and two less intense large peaks around 10 and 24°. The first fractions F₁ eluting during the column chromatography displays very similar diffraction pattern. The main peaks are almost the same with the most intense one at 2θ ≈ 7.47°. These three samples also share common peaks among the less intense ones. It can be noted that the peak at 12° was attributed to plane {001} of pyrene and its derivatives.³¹ The diffraction pattern is very different from the raw sample showing that the fractions F₁ present a more crystalline nature. The diffraction patterns of the second fractions F₂ have a few common peaks but are not very similar. F₄, in addition to the sharp peaks observed, displays underlying large peaks around less than 10° and 25° indicating the contribution of an amorphous phase. F₃ also displays underlying large peaks around less than 10° and 25° but few sharp peaks. The diffraction pattern of F₅ displays mainly quite large peaks around 10° and 20°. The fractions display really different diffraction pattern with the first ones exhibiting crystallinity and the last ones, especially F₅, a rather amorphous phase.

To perform in-depth structural characterization, scanning electron microscopy (SEM) and transmission electron microscopy (TEM) are presented in this section. Being organics samples, they charge up a lot under electron microscopy, which therefore produce white localized area. This is detrimental for the observations of the samples. Various aggregated structures were observed for the fractions obtained at the three different

<figure><img src="image_9.png" /><figcaption>Fig. 3 (a) Typical diffraction pattern obtained for the crude sample at the top and the diffraction pattern of the trinitropyrene (b) diffraction pattern of the fractions F₁ to F₅.</figcaption></figure>
<figure><img src="image_10.png" /></figure>

<figure><img src="image_11.png" /><figcaption>Fig. 4 SEM micrographs of the fractions F₁ (a), F₂ (b) and F₃ (c).</figcaption></figure>

durations, 20 min, 40 min and 60 min. In this paragraph, we
will only be discussing of the synthesis of 60 min duration (Fig.
4). The results for the 20 min and 40 min duration are available
in the ESI† (see S.I.F/†). The TEM micrographs are also dis-
cussed in the ESI (see S.I.G/)† For the 60 min, the fraction F₁ 60
min shows tangled, stacked thread-like structure of various size
(µm size) and diameter The sample charge up a lot so the
observation of the sample is difficult. Fraction F₂ 60 min
displays straight rods structure. F₃ 60 min shows irregular
sheets and sphere-shaped pieces. F₄ 60 min and F₅ 60 min
doesn't display any particular morphology. F₁ 60 min displays
similarities to the F₁ 20 min and F₁ 40 min whereas F₂ 60 min
morphology is quite different from F₂ 20 min and F₂ 40 min.
Overall, some fractions display quite regular structure. This
imply that the sample structure is organized on a long range.
This is in accordance with the XRD results that suggest that
these samples are crystalline. This is not something expected
for carbon dots but these morphologies are expected for organic
molecules. Moreover, the ability of pyrene derivatives that self-
assembled to form supramolecular object such as nanorods has
been reported.<sup>32-34</sup> This suggest, like the XRD and the HRMS
results, that the samples are more likely not exactly CDs.

Optical properties

The UV-vis spectra of the samples obtained after column chro-
matography and the trinitropyrene were recorded (Fig. 5). The
fractions are also compared between themselves for a given
duration or for a given fraction F<sub>n</sub> (see Fig. S.I.H/1 and S.I.J/1†).
For fraction F<sub>1</sub> and F<sub>2</sub>, pronounced absorption is observed at
around 400 and 500 nm. In the case of F<sub>3</sub>, its absorption bands
are slightly shifted at 430 and 530 nm with the 430 nm band
being significantly more intense than the 530. F<sub>4</sub> and F<sub>5</sub> displays
similar absorption bands to F<sub>3</sub>. However, for F<sub>4</sub>, the 530 band is
more intense than the 430 one and, for F<sub>5</sub>, both bands are of
similar intensity. Around 400 nm and 500 nm, significative
absorption bands are observed. F<sub>4</sub> and F<sub>5</sub> exhibit an absorption
band around 360 nm. Except for these two fractions, there is not
much absorption in the 300–400 nm area. Vibronic features and
quite sharp bands can be observed. It contrasts with the ex-
pected large UV-vis absorption for carbon dots and is consid-
ered characteristic of molecular fluorophores.<sup>35</sup> Moreover, the
absorbance spectra quite closely resemble the absorption
spectra of the trinitropyrene at the 400 nm region. Emission

spectra was also recorded. The small peak around 730 nm for
the TNP emission spectra is due to 2nd order scattering but
doesn't change the overall fluorescence of the TNP spectra.
From F₁ to F₄, brightly luminescence can be observed under 365
nm UV, lamp. The fraction F₅ also shows luminescence along-
side significant sedimentation at the bottom of the flask.
Fractions F₁ and F₂ have the similar maximum wavelength
emission of 618 nm. The maximum emission wavelength of F₃
is slightly shifted to the shorter wavelength. F₄ and F₅ differ with
a maximum wavelength emission of 580 nm. The 3D photo-
luminescence mapping of the fractions was also recorded. All
the fractions exhibit excitation-independent behaviour. This
suggests that the fractions are composed of one or more likely
a few similar fluorophores.

Discussion

The initial purpose of this experiment was to synthesize carbon
dots during microwave-assisted solvothermal treatment of tri-
nitropyrene. During this study, we observed that molecular
fluorophores are formed. The diffractogram of the crude sample
(Fig. 3(a)) obtained after the solvothermal treatment corre-
sponds to what is expected from carbon dots. In order to better
assess the composition of the sample, a chromatography
separation was executed inspired from a method previously
reported in the literature.³¹ After adding some adjustment to the
procedure, we sorted the initial sample in five different frac-
tions. Overall, the fractions obtained display similar photo-
luminescent properties but different structural properties (see
Table S.I.K/†). After characterization, the first four eluted frac-
tions are identified as molecular fluorophores. The last fraction
eluted, F₅, is strongly suggested as containing carbon entities,
likely carbon dots, and considered as the component that
initially leaded us to think that the crude sample contained
carbon dots based on the diffractogram. The molecular fluo-
rophores were isolated by column chromatography and, from
information obtained by characterization, we suggested that
they are small hydrophobic derivatives of nitropyrene. Indeed,
the FTIR and Raman characterization show the presence of
nitro group, aromatic double bond carbon and in-plane carbon
hydrogen bond in the different fractions. However, the less
intense peaks could not be attributed. The slight difference in
polarizability and optical properties could stem from these
subtle chemical differences. Even though fractions F₁ to F₄
<figure><img src="image_12.png" /></figure>

exhibited close hydrophobic behaviour, their distinct polariz-
ability allowed for their separation by chromatography. The
additional step in the chromatography step permitted a more
advanced separation based on the small difference in polariz-
ability of the fractions compared to the studies of Kothalawala
and Batra. They both used dichloromethane and methanol as
eluent for the column chromatography step whereas we used
cyclohexane, dichloromethane and methanol. Indeed, the
commonly used eluent system to separate hydrophobic
components for silica gel chromatography is constituted of
dichloromethane as the lower polarity eluent with methanol,
the higher polarity eluent. But, by adding a gradient of elution
using cyclohexane, an even lower polarity solvent than
dichloromethane, with dichloromethane allowed us to distin-
guish the first four fractions. Whereas, without this modifica-
tion, the first four fractions would have eluted together and we
would have ended up considering them as only one fraction.

Methanol was used with the intent to collect what didn't seem
to migrate with dichloromethane alone. Considering the fact
that the polarity strength of methanol is high, the first four
fractions could have eluted as one, had we not used cyclo-
hexane. The duration of the treatment was varied but no
significant changes in the nature and properties of the products
were observed in the range of duration studied. They display
similar product yield and quantum yield. The first four fractions
are distinguishable from the point of view of XRD and also SEM
to a lesser extent. However, they display little difference from
the point of view of spectroscopic techniques such as FTIR,
Raman spectroscopy, UV-vis absorption. Under SEM, some
fractions exhibit regular morphologies already encountered
with self-assembly of pyrene derivatives.³⁰⁻³⁴ Powder XRD
measurements suggests that samples organize in a quite
ordered crystalline form. However, parameters such as the
drying method, the type of solvents and the use of sonication

<figure><img src="image_13.png" /><figcaption>Fig. 5 (a) UV-vis absorbance spectra of the 5 fractions obtained for a 60 minute duration solvothermal treatment and TNP (b) photo-luminescence (λ<sub>ex</sub> = 470 nm) spectra of the 5 fractions obtained for a 60 minute duration solvothermal treatment and TNP. 3-D photoluminescence mapping of F<sub>1</sub> (c), F<sub>2</sub> (d), F<sub>3</sub> (e), F<sub>4</sub> (f), F<sub>5</sub> (g), and TNP (h) (coloured bars at the right display the photoluminescence counts per second).</figcaption></figure>
<figure><img src="image_14.png" /></figure>

are known to affect the formation of such supramolecular assemblies. Considering this, we cannot affirm that the samples that did not exhibit a clear morphology did so because the drying method was not adapted or they do not have a well-ordered morphology in powder form at all. F₅, with a proportion corresponding to approximately 10% of the sample, notably differs from the other fractions in particular by its significantly less pronounced hydrophobicity. Indeed, its elution during chromatography separation was only possible by drastically increasing the proportion of MeOH, hence the polarity of the eluent. The other fractions give clear solution in low polarity solvent even whereas solution obtained with fraction F₅ displays cloudy solution to a certain extent, with suspended particles. The results appeared to hint that the fraction F₅ contains or is composed of carbon entities such as carbon dots or carbon black and fluorophores free or attached to the nanoparticles. The results from the mass spectrometry analysis indicates that, even though the diffraction pattern is similar to what is expected from carbon dots, this sample could be composed of nitropyrene derivatives that differ from the other fraction that grant it a higher polarizability. The fact that it appears as an amorphous sample may be attributed to the drying process or an inherent inability to self-organize in an ordered form compared to the other fractions. Pyrene derivatives are of particular interest in supramolecular chemistry as building blocks for self-assembling. Indeed, their self-assembly behaviour in structures such as nanorods and there notable optical and electronic properties make them interesting candidates for research in this field.³⁶ Through π-π stacking, nanostructures such as nanorods and nanowires were produced, because this type of interaction involves relatively high energy (ca. 10-70 kJ mol⁻¹) and is highly directional. Templates are however needed in order to improve the crystallinity.³⁷,³⁸ Hence, studies are focusing on preparing building blocks that exhibit well-ordered self-assembly. Some studies also obtained organic nanoparticles identified as molecular fluorophores employing other precursor material than trinitropyrene like citric acid.³⁹⁻⁴¹ This contributed to warning future studies that carefulness is necessary when evaluating samples obtained by a method commonly used to synthesize carbon dots. Though serendipitously, this study brings some information on a synthesis of luminescent self-assembling structures that displays crystallinity to a certain extent. Moreover, their hydrophobicity endows the fractions F₁ to F₄ great solubility in low polarity solvents. This feature and their luminescent properties could be used in ordered to prepare luminescent materials blending them in polymers such as polystyrene.

## Conclusions

Altogether, this study shows that molecules with significant fluorescent properties are produced during the solvothermal treatment of trinitropyrene. These fluorophores are highly emissive and responsible for most of the luminescence observed. Several fractions of molecular fluorophores were isolated through advanced purification steps and characterized in an attempt to identify their structures. The fractions isolated

displayed similar photoluminescent properties and chemical composition but significant dissimilarities were observed from a structural point of view. Some fractions exhibited crystalline diffraction pattern, defined morphologies whereas some other samples do not show any particularly defined morphology. Molecular fluorophores were associated with derivatives of trinitropyrene, the precursor material and are thought to be mainly responsible for the luminescence fluorescence observed. This works aims to contribute to the understanding of the formation of fluorophores from a popular carbon dots precursor, trinitropyrene, used in solvothermal conditions.

## Data availability

Data supporting this article, including HRMS spectra, UV-vis absorbance spectra, Fluorescence emission spectra, FTIR spectra, Raman spectra, XRD diffraction patterns, SEM micrographs, have been included as part of the ESI.†

## Author contributions

Rayan Roch: data curation, investigation, methodology, writing – original draft, conceptualization, formal analysis. Xavier Deschanels: supervision, validation, writing – review & editing. Chandra Mohan Singaravelu: conceptualization, supervision, formal analysis. Noé André: formal analysis. Cyrielle Rey: formal analysis, supervision. Jérémy Causse: supervision, conceptualization, investigation, methodology, project administration, resources, validation, writing – review & editing.

## Conflicts of interest

There are no conflicts to declare.

## Acknowledgements

The authors would like to thank Magalie Lefeuvre from the University of Montpellier for the help and support for HRMS measurements, Joseph Lautru for his help in SEM measurements and Olivier Gueton for fruitful discussions.

## Notes and references

1. X. Xu, R. Ray, Y. Gu, H. J. Ploehn, L. Gearheart, K. Raker and W. A. Scrivens, *J. Am. Chem. Soc.*, 2004, **126**, 12736-12737.

2. V. Michaud, J. Pracht, F. Schilfarth, C. Damm, B. Platzer, P. Haines, C. Harreiß, D. M. Guldi, E. Spiecker and W. Peukert, *Nanoscale*, 2021, **13**, 13116-13128.

3. D. Lu, K. Yin, Y. Zhao, Z. Gao, N. Godbert, H. Li, H. Li and J. Hao, *Colloids Surf.*, A, 2021, **613**, 126129.

4. B. Wang, W. Luo, D. Wu, S. Li and F. Geng, *Spectrochim. Acta, Part A*, 2023, **303**, 123117.

5. B. Liu, J. Tao, J. Pan, C. Li, F. Li and Y. Zheng, *Opt. Mater.*, 2021, **113**, 110892.

6. X. Chang, G. Zhao, C. Liu, X. Wang, A. M. A. Abdulkhaleq, J. Zhang and X. Zhou, *RSC Adv.*, 2022, **12**, 28021-28033.
<figure><img src="image_15.png" /></figure>

7 C. Wang, C. Pan, Z. Wei, J. Liu, Z. Song, W. Ma, M. Wang and L. Mao, *Microchim. Acta*, **2021**, *188*, 330.

8 M. Tepakidareekul, T. Uematsu and S. Kuwabata, *RSC Adv.*, **2022**, *12*, 20054–20061.

9 F.-J. Cao, X. Hou, K.-F. Wang, T.-Z. Jin and H. Feng, *RSC Adv.*, **2023**, *13*, 21088–21095.

10 F. Yuan, T. Yuan, L. Sui, Z. Wang, Z. Xi, Y. Li, X. Li, L. Fan, Z. Tan, A. Chen, M. Jin and S. Yang, *Nat. Commun.*, **2018**, *9*, 2249.

11 F. Yuan, Y.-K. Wang, G. Sharma, Y. Dong, X. Zheng, P. Li, A. Johnston, G. Bappi, J. Z. Fan, H. Kung, B. Chen, M. I. Saidaminov, K. Singh, O. Voznyy, O. M. Bakr, Z.-H. Lu and E. H. Sargent, *Nat. Photonics*, **2020**, *14*, 171–176.

12 J. Guo, Y. Lu, A.-Q. Xie, G. Li, Z.-B. Liang, C.-F. Wang, X. Yang and S. Chen, *Adv. Funct. Mater.*, **2022**, *32*, 2110393.

13 J. Deng, Q. Lu, N. Mi, H. Li, M. Liu, M. Xu, L. Tan, Q. Xie, Y. Zhang and S. Yao, *Chem.-Eur. J.*, **2014**, *20*, 4993–4999.

14 Q. An, Q. Lin, X. Huang, R. Zhou, X. Guo, W. Xu, S. Wang, D. Xu and H.-T. Chang, *Dyes Pigm.*, **2021**, *185*, 108878.

15 Y.-S. Lee, C.-C. Hu and T.-C. Chiu, *J. Environ. Chem. Eng.*, **2022**, *10*, 107413.

16 D. Qu and Z. Sun, *Mater. Chem. Front.*, **2020**, *4*, 400–420.

17 S. Xue, P. Li, L. Sun, L. An, D. Qu, X. Wang and Z. Sun, *Small*, **2023**, 2206180.

18 L. Wang, Y. Wang, T. Xu, H. Liao, C. Yao, Y. Liu, Z. Li, Z. Chen, D. Pan, L. Sun and M. Wu, *Nat. Commun.*, **2014**, *5*, 5357.

19 L. Wang, W. Li, B. Wu, Z. Li, D. Pan and M. Wu, *Chem. Eng. J.*, **2017**, *309*, 374–380.

20 M. Wu, J. Zhan, B. Geng, P. He, K. Wu, L. Wang, G. Xu, Z. Li, L. Yin and D. Pan, *Nanoscale*, **2017**, *9*, 13195–13202.

21 J. Zhan, B. Geng, K. Wu, G. Xu, L. Wang, R. Guo, B. Lei, F. Zheng, D. Pan and M. Wu, *Carbon*, **2018**, *130*, 153–163.

22 W. Li, M. Li, Y. Liu, D. Pan, Z. Li, L. Wang and M. Wu, *ACS Appl. Nano Mater.*, **2018**, *1*, 1623–1630.

23 B. Geng, D. Yang, D. Pan, L. Wang, F. Zheng, W. Shen, C. Zhang and X. Li, *Carbon*, **2018**, *134*, 153–162.

24 R.-S. Juang, C.-T. Hsieh, C.-P. Kao, Y. A. Gandomi, C.-C. Fu, S.-H. Liu and S. Gu, *Carbon*, **2021**, *176*, 61–70.

25 K.-B. Cai, H.-Y. Huang, M.-L. Hsieh, P.-W. Chen, S.-E. Chiang, S. H. Chang, J.-L. Shen, W.-R. Liu and C.-T. Yuan, *ACS Nano*, **2022**, *16*, 3994–4003.

26 Y. Li, H. Li and Y. Xu, *ChemistrySelect*, **2023**, *8*, e202204013.

27 G. Liu, M. Zavelani-Rossi, G. Han, H. Zhao and A. Vomiero, *J. Mater. Chem. A*, **2023**, *11*, 8950–8960.

28 X. Zhang, Z. Liu, H. Guo, C. Chen, Z. Zeng, J. Xu and L. Wang, *ChemNanoMat*, **2023**, e202300187.

29 C.-C. Hsu, L. Laysandra, Y.-C. Chiu and W.-R. Liu, *Chem. Eng. J.*, **2023**, *473*, 145469.

30 G. Batra, S. Sharma, K. Kaushik, C. Rao, P. Kumar, K. Kumar, S. Ghosh, D. Jariwala, E. A. Stach, A. Yadav and C. K. Nandi, *Nanoscale*, **2022**, *14*, 3568–3578.

31 N. L. Kothalawala, S. W. Kim, N. Kim, C. J. Henderson, M. Seol, F. Yang, S.-Y. Kwak, K. Y. Hwang, W.-J. Son, H.-J. Shin, H. Choi, B.-S. Kim and D. Y. Kim, *New J. Chem.*, **2022**, *46*, 8324–8333.

32 M. E. Idrissi, S. J. Teat, P. F.-X. Corvini, M. J. Paterson, S. J. Dalgarno and P. Shahgaldian, *Chem. Commun.*, **2017**, *53*, 1973–1976.

33 R. P. Bhatta, V. Kachwal, C. Climent, M. Joshi, P. Alemany, A. R. Choudhury and I. R. Laskar, *J. Mater. Chem. C*, **2023**, *11*, 11399–11408.

34 Y.-F. Li, X. Wang, C.-Y. Wang, Y. Wang and Y.-W. Yang, *Tetrahedron*, **2023**, *149*, 133718.

35 V. Hinterberger, C. Damm, P. Haines, D. M. Guldi and W. Peukert, *Nanoscale*, **2019**, *11*, 8464–8474.

36 B.-Q. Ma and P. Coppens, *Chem. Commun.*, **2003**, 2290.

37 X. Zhang, X. Zhang, W. Shi, X. Meng, C. Lee and S. Lee, *J. Phys. Chem. B*, **2005**, *109*, 18777–18780.

38 Z. Wang, Y. Xie and C. Gao, *RSC Adv.*, **2012**, *2*, 11354.

39 J. Zhang, L. Yang, Y. Yuan, J. Jiang and S.-H. Yu, *Chem. Mater.*, **2016**, *28*, 4367–4374.

40 C. J. Reckmeier, J. Schneider, Y. Xiong, J. Häusler, P. Kasák, W. Schnick and A. L. Rogach, *Chem. Mater.*, **2017**, *29*, 10352–10361.

41 J. Yang, L. Guo, X. Yong, T. Zhang, B. Wang, H. Song, Y. Zhao, H. Hou, B. Yang, J. Ding and S. Lu, *Angew. Chem., Int. Ed.*, **2022**, *61*(33), e202207817.